Biopolymer based nanomaterials as potential biosorbents for toxic metal ions
Chemical and Process Engineering Research www.iiste.orgISSN 2224-7467 (Paper) ISSN 2225-0913 (Online)Vol.11, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications7Biopolymer Based Nanomaterials as Potential Biosorbents forToxic Metal Ions1. Asma Sadiq1 *,Anita Choubey1, Leena Rai 2and A.K.Bajpai2Department of Chemistry, Govt. M.L.B.College, Bhopal MP2. Bose Memorial Research LaboratoryDepartment of Chemistry, Government Autonomous Science College, Jabalpur MPABSTRACTIn the present work ternary nanoparticles of chitosan, yeast and gelatin were prepared by emulsion crosslinkingmethod and characterized by techniques like FTIR and TEM. Whereas the spectral studies confirm the presenceof characteristic functional groups of the three biopolymers. The TEM analysis also reveal that the size ofnanoparticles lie in the range 50 to 150 nm. The nanospheres so prepared were examined for removal of Cu (II)ions and it was found that the removal capacity of metal ions was more than 90 percent. The metal ion removalcapacity of the nanoparticles was found to depend on the chemical composition of the adsorbent, concentrationof the metal ion solution, pH and temperature of the medium and agitation speed of the suspension.* Presenting AuthorINTRODUCTIONClean water (i.e. water free of toxic chemicals and pathogens) is essential to human health. Clean wateris also a critical feedstock in a variety of key industries including electronics, pharmaceuticals, metallurgical andfood. The world is facing formidable challenges in meeting rising demand of clean water as the availablesupplies of fresh water are decreasing due to extended droughts, population growth, competing demands from avariety of users, etc1.Sachromyces cerevisiae (yeast) is readily available biopolymer used for removal of heavy metal ionssuch as Cu2+, Cd2+, Pb2+, Zn2+, Cr2+and Ni2+. The use of chelation while the harmless ions move on into theenvironment. Some of the known ion–exchange materials consist of different biopolymers like cellulose,alginates, proteins, chitin and chitin derivatives, etc. Among these biopolymeric materials chitosan has a primerank as adsorbent for removal of toxic metal ions. Chitosan is a heteropolymer made of D–glucosamine and asmall fraction of N–acetyl–D–glucosamine residues. Thus, due to the presence of free reactive amino group inchitosan it rapidly undergoes complex formation between metal ion and the polymer. The present study aims atinvestigating the removal of Cu2+ions from aqueous solution by adsorption onto the nanoparticles composed ofchitosan, gelatin and yeast. Copper being the most widely used heavy metal is mainly employed in electrical andelectroplating industries and in large amount is extremely toxic for living organisms. The presence of copper (II)ions causes serious toxicological concern, which is usually known to deposit in brain, skin, liver, pancreas andmyocardium.EXPERIMENTALMaterialsBiopolymers like chitosan, yeast, gelatin (Loba Chemie, India) . Glutaraldehyde (Loba Chemie,Mumbai, India was used as crosslinking agent. Silicon oil (Aldrich, USA) viscosity 10,000 (at 25oC) was used asan oil phase for preparing the suspension. Copper sulphate and other chemicals were of high purity grade andthroughout the work; double distilled water was used for making solutions.MethodsPreparation of NanospheresA known solution of gelatin (3 g) and yeast (2 g) were mixed with a known solution of chitosan (1 g) onmagnetic stirrer for about 20 min. 3 mL homogeneous mixture of glutaraldehyde and silicon oil was addeddropwise into the suspension of yeast, gelatin and chitosan with the help of a syringe under constant stirring.Prepared nanoparticles were washed with acetone, then benzene and dried at 80oC for 2–3 h.Adsorption ExperimentsThe adsorption was carried out by the batch contact method as described elsewhere 2. In brief, the stocksolution was prepared by dissolving 0.6 g of copper sulphate in 1 liter distilled water. In to 6 mL of diluted stocksolution (1:1), 100 mg of swollen nanospheres were added as adsorbent. The suspension was shaken in a rotaryshaker (Tempstar, India) for 4 h which was found to be a sufficient time to attain equilibrium adsorption. Aftershaking is over, 3 mL supernatant was mixed with 1 mL reagent (NH3 solution) and the amount of copper wasassayed spetrophotometrically. The adsorbed Cu (II) was calculated by the following mass balance equation,where Ci and Cf being the initial and final concentrations of CuSO4 solution (mg/mL). V being the volume of
Chemical and Process Engineering Research www.iiste.orgISSN 2224-7467 (Paper) ISSN 2225-0913 (Online)Vol.11, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications8adsorbed solution and m is the weight of swollen nanospheres, i.e. adsorbent.FTIR Spectral AnalysisThe FTIR spectra of native (unadsorbed) and Cu (II) adsorbed nanospheres were recorded on a FTIRspectrophotometer (FTIR–8400S, Shimadzu).Transmission Electron Micrograph (TEM)In order to study morphology of the prepared nanospheres, the TEM analysis of the microspheressurface was carried out (STEREO SCAN, 430, Leica , USA).RESULTS AND DISCUSSIONFTIR AnalysisThe FTIR spectra of both native and Cu2+adsorbed biopolymeric nanospheres are shown in Fig. 1(a)and (b), respectively. Whereas, the spectrum (a) confirms the presence of the biopolymer components, i.e.chitosan, yeast and gelatin in the nanospheres, the spectra (b) also indicate the sorption of Cu2+ions into thenanospheres. The IR spectrum of nanospheres [Fig. 1(a)] shows peak around1171 cm–1corresponding tosaccharide structure25. A sharp peak appearing at 1615 cm–1may be attributed to amide I band (nC=O),characteristic of chitosan with acetylated unit. A cluster of peaks around 3422 cm–1may be assigned tooverlapped absorption bands due to N–H and O–H symmetrical vibrations. Peaks around 2910 cm–1are thetypical C–H stretch vibrations.A close examination of spectrum (b) reveals that several specific bands appearedat 1615 cm–1, 2910 cm–1and 3422 cm–1are shifted to longer wave numbers at 1683 cm–1, 2940 cm–1and 3544cm–1, respectively due to interaction of metal ions (Cu2+) with biopolymer components.Fig. 1: FTIR spectra of nanosphere Fig. 2: TEM image of prepared nanospheresTransmission Electron Micrograph (TEM)The TEM image of the nanospheres surfaces is shown in Fig. 2 which clearly indicates that the threecomponents (yeast, gelatin, chitosan) of the nanospheres are very compatible to each other. Therefore, thesurface appears quit homogeneous and even. The size of nanospheres varies from 30 to 150 nm.Langmuir IsothermEquilibrium studies that give the capacity of the adsorbent and adsorbate are described by adsorptionisotherm which is usually the relation between quantity adsorbed and that remaining in solution at fixedAdosrbed amount (mg/g) =(Ci – Cf) Vm... (1)
Chemical and Process Engineering Research www.iiste.orgISSN 2224-7467 (Paper) ISSN 2225-0913 (Online)Vol.11, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications9temperature at equilibrium. The most common type is the Langmuir 3isotherm as shown in Fig. 3.Figure 3 Langmuir adsorption isotherm plot Fig. 4 Effect of chitosan on adsorptionWhere a is the adsorbed amount of Cu2+(mg/g) at any equilibrium concentration, as is the adsorbedamount of metal ion at saturation (adsorption capacity), K is the adsorption coefficient which is equal to k1/k2,where k1 and k2 are rate constants for the adsorption and desorption, respectively. The linear plot of Ce/a vs Ceshows that adsorption follow Langmuir adsorption. The values of as and K may be determined from the slopeand intercept values and found to be 250 mg/g–1and 0.2 (mg–1dm3), respectively.(i) Effect of ChitosanWhen chitosan is varied in the range 0.5 g to 2.0 g, adsorption of Cu2+ions varies as shown in Fig.4.The results clearly show that with increasing concentration of chitosan, adsorption initially increases and thendecreases. The results may be explained by the fact that amino sugar of chitosan and chitin are major effectivebinding sites for metal ion and form stable complex with metal ions by co–ordination.Thus, obviously with increasing chitosan content in the nanospheres, the adsorption of metal ions alsoincreases, whereas beyond an optimum concentration of chitosan (1.0 g) the observed decrease may be attributedto the reason that at higher chitosan content, the intermolecular forces become much stronger and this causesshrinkage in the pore size of the nanospheres. This clearly results in a fall in the adsorbed metal ionsFig. 5 Effect of gelatin on adsorption of metal ions Fig. 6 Effect of yeast on adsorption of copper(ii) Effect of GelatinIn the case of gelatin, the amount was varied in the range of 2.0 g to 3.5 g. The results shown in Fig. 5indicate that the adsorption of Cu2+increases with increasing gelatin concentration up to 3.0 g and then increaseCe=a as K as1 Ce+ ... (3)
Chemical and Process Engineering Research www.iiste.orgISSN 2224-7467 (Paper) ISSN 2225-0913 (Online)Vol.11, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications10in gelatin concentration results in a decrease in the adsorption.(iii) Effect of YeastIn the case of yeast, the variation in the amount was in the range 1.0 g to 2.5 g. The results are shown inFig. 6 which reveals that the adsorption of Cu2+ions increases with increasing yeast concentration up to 3.0 gand then further increase in yeast concentration results in a decrease in the adsorption.Effect of pHpH seems to be the most important parameter in the biosorption process. It affects the solutionchemistry of the metal ion, the activity of the functional groups in the biomass and competition of metallic ions.Cu2+exhibits different type of pH dependence equilibria in aqueous solution. As pH is shifted the equilibriumwill also shift. The effect of pH on the adsorbed amount of Cu2+ions have been investigated in the range 1.2 to 5as shown in Fig. 7. Effect of Temperature. In the present work, the effect of temperature on adsorption was studied in the range 5o–40oC. Theresults are shown in Fig. 9 which indicates that adsorption increases from 5 to 22oC and then starts decreasing.Fig. 7 Effect of pH on adsorption Fig. 8 Influence of temperatureCONCLUSIONSChemical crosslinking of a water/oil suspension of a gelatin, yeast and chitosan produces regularshaped nanospheres of size up to 150 nm. The prepared nanospheres show potential for the removal of Cu2+ionsfrom aqueous solutions.The adsorption of Cu2+ions onto the water–swollen nanospheres increases with increasing initial metalion concentration in the range 1.0 to 8.0 mg/mL. It is noticed that in the higher concentration range (8 mg/mL),the adsorbed amount nearly levels off. The adsorption process is found to follow Langmuir adsorption isothermsequation characterized by the appearance of a well marked plateau portion. The adsorption of Cu2+ionsalso exhibits a significant change with changing concentration of the nanospheres biopolymeric constituents. It isobserved that there is a definite concentration of chitosan, gelatin and yeast at which the adsorption of Cu2+ionsis optimum and on both the sides of this optimum concentration, the adsorption is comparatively low. Theadsorbed amount of Cu2+ions is significantly affected by pH of the metal ion solution when varied in the range1.2 to 5.4. It is noticed that the adsorbed amount steeply increases in the range 1.2 to 2.4 while a marginalincrease occurs beyond pH 2.4. An optimum amount of Cu2+ion is adsorbed at 25oC while it decreases on boththe sides of this temperature.REFERENCES1. Savage N, Diallo MS. Nanomaterials and water purification: opportunities and challenges. JNanoparticle Res 2005; 7:325-330..2. Bajpai AK, Sachdeva R. Adsorption of casein onto alkali treated bentonite. J Appl Polym Sci 2000;78:1656-1663.3. Pinghe-Yin, Caiming Yu, Bo Jin, Zhao Ling. Biosorption removal of cadmium from aqueous solutionby using pretreated fungal biomass cultured from starch waste water. Water Res 1999; 33(8):1960-1963.
This academic article was published by The International Institute for Science,Technology and Education (IISTE). The IISTE is a pioneer in the Open AccessPublishing service based in the U.S. and Europe. The aim of the institute isAccelerating Global Knowledge Sharing.More information about the publisher can be found in the IISTE’s homepage:http://www.iiste.orgCALL FOR PAPERSThe IISTE is currently hosting more than 30 peer-reviewed academic journals andcollaborating with academic institutions around the world. There’s no deadline forsubmission. Prospective authors of IISTE journals can find the submissioninstruction on the following page: http://www.iiste.org/Journals/The IISTE editorial team promises to the review and publish all the qualifiedsubmissions in a fast manner. All the journals articles are available online to thereaders all over the world without financial, legal, or technical barriers other thanthose inseparable from gaining access to the internet itself. Printed version of thejournals is also available upon request of readers and authors.IISTE Knowledge Sharing PartnersEBSCO, Index Copernicus, Ulrichs Periodicals Directory, JournalTOCS, PKP OpenArchives Harvester, Bielefeld Academic Search Engine, ElektronischeZeitschriftenbibliothek EZB, Open J-Gate, OCLC WorldCat, Universe DigtialLibrary , NewJour, Google Scholar